Phase Transformation in Super Elastic NiTi Polycrystalline Micro-tubes Under Tension and Torsion -...
Embed Size (px)
Transcript of Phase Transformation in Super Elastic NiTi Polycrystalline Micro-tubes Under Tension and Torsion -...
International Journal of Solids and Structures 39 (2002) 37973809 www.elsevier.com/locate/ijsolstr
Phase transformation in superelastic NiTi polycrystalline micro-tubes under tension and torsionfrom localization to homogeneous deformationQing-Ping Sun *, Zhi-Qi LiDepartment of Mechanical Engineering, The Hong Kong University of Science and Technology, Clear Water Bay, Kowloon, Hong Kong SAR, PR China
Abstract Recent tensiontorsion test results on nano-grained NiTi shape memory alloy micro-tubes are reported in this paper. It is discovered that: (1) during uniaxial tensile loading, the stress-induced transformation in the micro-tubes is realized by the initiation and growth of a macroscopic spiral martensite band with a quite sharp austenitemartensite (AM) interface; (2) during loading by torsion (pure shear), the stressstrain curve exhibits monotonic hardening, the stressinduced transformation is axially homogeneous throughout the whole tube and the transformation strain is much smaller than that under tension; (3) under tensiontorsion combined loading with an increasing shear/tension stress ratio, there is a gradual change in the deformation mode from localization and propagation (under pure tension) to the homogeneous deformation (under pure shear). The tube surface morphology observation indicates that, during this gradual change, the AM interface thickness increases as its evolution is recorded. The test results demonstrate that there is a strong anisotropy and loading path dependence of the tube responses in both kinematics and kinetics. Possible underlying physical mechanisms are analyzed and implications for future theoretical modelling are also discussed. 2002 Elsevier Science Ltd. All rights reserved.Keywords: Phase transformation; NiTi shape memory alloy micro-tubes; Tension/torsion test; Material instability; Thickness of AM interface
1. Introduction Applications of shape memory alloys (SMAs) in the medical industry are multiplying rapidly. NiTi polycrystalline SMAs, due to their unique superelastic properties and biocompatibility, have been successfully used as components of medical devices in recent years. An outstanding example is of their use in minimal access surgery and less invasive operations as guidewires, guidetubes and stents. The high exibility, large recoverable deformation, good fatigue life and outstanding superelastic behavior at or around body temperature of NiTi superelastic tubes and wires make it possible to minimize the size of critical
Corresponding author. Tel.: +852-2358-8655; fax: +852-2358-1543. E-mail address: firstname.lastname@example.org (Q.-P. Sun).
0020-7683/02/$ - see front matter 2002 Elsevier Science Ltd. All rights reserved. PII: S 0 0 2 0 - 7 6 8 3 ( 0 2 ) 0 0 1 8 2 - 8
Q.-P. Sun, Z.-Q. Li / International Journal of Solids and Structures 39 (2002) 37973809
medical devices and to perform functions that would be impossible with other materials. High mechanical reliability (such as kink resistance) and controllability of the deformation of the devices (via stress/temperature-induced phase transitions) are two critical requirements of very long and small-diameter surgical instruments (allowing push/pull/twist manipulations) (Duerig, 1995; Pelton et al., 1997). These requirements are dependent upon the constitutive behavior of the material under complex loading conditions. Experimental investigation on NiTi micro-tube materials has been conducted in recent years and some preliminary results have been obtained (see Pelton et al., 1997; Sun et al., 2000; Li and Sun, 2002). Fundamental mechanics studies on the behavior and modelling of bulk superelastic NiTi wires and strips have attracted a lot of research attention in the past decade (for example see Abeyaratne and Knowles, 1990, 1993; Shaw and Kyriakides, 1995, 1997, among many others). In recent years, the eect of texture and microstructure anisotropy on the constitutive behavior of SMAs has become an issue of interest and has been investigated by many researchers (for example, the work of Thamburaja and Anand (2001), Shu and Bhattacharya (1998), Miyazaki et al. (2000), Gall and Sehitoglu (1999), Patoor et al. (2001), Sittner and Novak (2000), Liu et al. (1999) and Song et al. (2000a,b)). The micro-tubes are typically obtained by drawing process during which severe plastic deformation happened and a strong crystalline texture may develop in the tubes. Therefore the micro-tube samples make it possible to combine biaxial test with material anisotropy test. Experimental investigation to understand the fundamental mechanics of nanograined NiTi micro-tube materials has not yet been reported. Test data for critical comparisons with exiting theoretical modelling are lacking. This paper reports on an experimental study of the constitutive behavior of polycrystalline NiTi microtube material under tension, torsion and tension/torsion combined loadings. The main objective of this work is to reveal the eect of external stress states as well as internal microstructures on the macroscopic behavior of the material during phase transformation. The specimen preparation and experimental procedures are described in Section 2 and the results of uniaxial tension are briey reported in Section 3. In Section 4, the results under pure torsion and torsion/tension combined loading tests are reported. Macroscopic nominal stressstrain curves under dierent tension/torsion loading ratios are measured and presented. Quantitative surface morphology observations are also reported on the material under dierent loading conditions, especially in regards to variations in the austenitemartensite (AM) interface thickness during the loading. The results are discussed in Section 5 in which issues regarding the underlying mechanisms and the theoretical modelling of the observed phenomena are addressed.
2. Experimental procedures 2.1. Material The micro-tubes are commercially available (Shape Memory Application, Inc., USA) polycrystalline NiTi with grain sizes of 3050 nm. Micro-tubes of two sizes are used in the test: one with an outer diameter of 1.12 mm and other of 1.5 mm. The usual thickness/diameter (t=D) ratios for both tubes are 10%. In the tests of each tube diameter, all specimens are cut from a single tube in order to reduce uctuations in material properties. The composition (provided by the manufacturer) and the transition temperatures of the materials (measured by a dierential scanning calorimeter, DSC) are shown in Table 1. At room temperature (23 C), the superelastic behavior of the material is guaranteed. During loading, austenite loses its stability and stress-induced martensite begins to form. During unloading, the stress-induced martensite becomes unstable and transforms back to austenite. Fig. 1(a) shows schematically the mechanical cold-drawing process of NiTi micro-tubes. Tubes were drawn through dies using a guide bar to keep them straight and to give the nal inner diameter. The outer diameter and thickness of the tubes are thus reduced and signicant plastic deformation takes place. During
Q.-P. Sun, Z.-Q. Li / International Journal of Solids and Structures 39 (2002) 37973809 Table 1 Composition (wt.%) and transition temperatures (C) of the tube materials Ni (%) 1.12 mm tube 1.5 mm tube 51 56 Ti (%) 49 44 As (C) 2.69 3.26 Af (C) 22.4 17.4 Ms (C) 56.3 54.2 Mf (C) 77.6 67.6
Fig. 1. (a) Schematic illustration of drawing process, (b) TEM picture of grain size of the tube (arrow shows the drawing direction) and (c) TEM picture of grain size of the wire (1.3 mm diameter) for comparison.
the drawing process, strong crystalline texture develops due to the rotation of the slip systems in the grains. To observe the microstructure of the material, a slice is cut along the axis direction of the tube. Fig. 1(b) shows a typical microstructure of the tube (grain sizes about 50100 nm) by transmission electron microscopy (TEM). Fig. 1(c) is the TEM photo of a much less deformed drawn wire (1.3 mm diameter) for comparison. It is seen that there exists a strong texture in the tubes because of the severe plastic deformation during cold drawing. This contributes to signicant anisotropy in the transformation behaviors between tension and torsion as shown in the following sections.
Q.-P. Sun, Z.-Q. Li / International Journal of Solids and Structures 39 (2002) 37973809
Fig. 2. The grips and the way to load the tube under (a) pure tension and (b) pure torsion.
2.2. Experiment set-up (i) Uniaxial tension test. The experiments were conducted at room temperature (23 C) in a standard testing machine (Sintech 10D with a 1 KN load cell) under displacement control. To clamp the tube for the tension and torsion tests and to eliminate the stress concentration in the clamped area, a special grip for thin-walled micro-tubes was designed as shown in Fig. 2(a). The blocks on which the tubes are adhered are connected to the test machine by two two-pin hinge connectors. This type of grip, which transfers a concentrated force at the end of cylinder into a uniform axial shear stress on the tube surface at the two ends, is very eective in removing the bending and torsion caused by the clamps eccentricity. The tubes are bonded to the block by an epoxy (plastic welding system, no. 47809, shear strength at room temperature 3500 psi). The bonded length of each tube is 20 mm at each end. An extensometer is used to measure the tube elongation and nominal strain. In order to hold the extensometer, two additional plates are xed to the blocks by screws. In this way, the eective gauge length is 52 mm (Fig. 2). (ii) Torsion and tension/torsion tests. The responses of the tubes under torsion and tension/torsion were measured at room temperature (23 C) in a standard testing machine together with a specially designed torsion loading device. The c